Issue 
EPJ Photovolt.
Volume 9, 2018



Article Number  11  
Number of page(s)  6  
Section  Modelling  
DOI  https://doi.org/10.1051/epjpv/2018009  
Published online  30 November 2018 
https://doi.org/10.1051/epjpv/2018009
Regular Article
Beneficial impact of a thin tunnel barrier in quantum well intermediateband solar cell
^{1}
Aix Marseille Université, CNRS, Université de Toulon, IM2NP UMR 7334,
13397
Marseille, France
^{2}
NextPV, LIA, CNRSRCAST/U, TokyoU, Bordeaux,
Tokyo
1538904, Japan
^{3}
Research Center for Advanced Science and Technology, The University of Tokyo,
Tokyo
1538904, Japan
^{4}
LIMMS, CNRSInstitute of Industrial Science, UMI 2820, University of Tokyo,
Tokyo
1538505, Japan
^{5}
IRDEP, UMR 7174 CNRS EDF Chimie ParisTech, EDF R&D,
Chatou, France
^{*} email: nicolas.cavassilas@im2np.fr
Received:
25
July
2018
Received in final form:
16
October
2018
Accepted:
19
October
2018
Published online: 30 November 2018
Based on electronic quantum transport modeling, we study the transition between the intermediateband and the conductionband in nanostructured intermediateband solar cell. We show that a tunnel barrier between the quantum well (QW) and the host material could improve the current. The confinement generated by such a barrier favors the intersubband optical coupling in the QW and then changes the excitationcollection tradeoff. More surprisingly, we also show that tunneling impacts the radiative recombination and then the voltage. Using a detailed balance model we explain and we propose a broadening factor for this V_{oc} modification. Finally we show that a thin tunnel barrier is beneficial for both current and voltage.
Key words: intermediate band solar cell / quantum modeling / quantum structures / intraband transition
© N. Cavassilas et al., published by EDP Sciences, 2018
This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
1 Introduction
By introducing an intermediate band (IB) in a wide bandgap solar cell, the aim is to increase the short circuit current I_{sc} without reducing the opencircuit voltage V_{oc} [1,2]. The current increases as the IB acts as a built in upconverter to generate an electron hole pair with two lowenergy photons. To limit detrimental effect voltage drop, the IB must be electrically isolated from the contacts of the cell so that the recombination is still controlled by the wide bandgap. This theoretically allows to exceed the Shockley–Queisser (SQ) efficiency limit [3] with a V_{oc} controlled by the wide bandgap while lowenergy photons generate electronhole pairs.
Yet practically, this concept has not yet resulted in a cell exceeding the SQ limit [4,5]. However, IB solar cell (IBSC), generally based on quantum structures, still offers characteristics that are often lower than that of the same cells without IB [6]. To address this issue the increase of current [7] is not enough to catch up with the degradation of the V_{oc}. It is difficult to obtain a splitting between the Fermi levels of the IB and the contact (usually the ntype contact) because the electrons easily relax from the conduction band of the wide bandgap material to the IB. In other words, the IB is not well isolated from contacts and V_{oc} is controlled by recombination across a narrow bandgap.
Furthermore, the increase of current remains low as it is difficult to have simultaneous efficient photon absorption and a fast collection of the excited electrons. Indeed, if the IBSC is based on quantum structures, the electrons in IB are confined in localized states. The optical transition between the IB and the conduction band is then efficient if the excited state is also localized. This improves the wavefunction overlap and the corresponding intraband (intersubband) transition [8,9]. However, if the excited electron is strongly confined in the quantum structure, it cannot reach the conduction band to be collected. It will finally relax by emitting photon and/or phonons. As a result the choice of the coupling between the excited state of the quantum structures and the conduction band of the wide bandgap is crucial to have a good excitationcollection tradeoff. In case of boundtobound absorption with a thick tunnel barrier the absorption is high, but the electrons collection is limited. In a boundtocontinuum absorption without tunnel barrier the collection is fast but the absorption is low. In this letter we propose a comprehensive analysis of this problem. We will see that a thin tunneling barrier between the quantum structure and the wide bandgap material offers a good excitationcollection tradeoff. This permits to optimize the current generated by the intraband transition of an IBSC. More unexpected, we will show that such a coupling also modifies the photon emission in the intraband transition and then impacts the V_{oc}.
2 Model and system
This theoretical study is based on a quantum electronic transport model in the nonequilibrium Green functions (NEGF) framework. This model allows to consider the quantum effects, such as the confinement, the tunneling, the broadening due to the coupling and the scattering with the photons and the phonons. Nevertheless, except when this will be explicitly stated, we will not consider scattering with phonons. Such a radiative limit permits to facilitate the understanding of the results. The model used is described in reference [10] but as suggested in reference [11] we now consider the nonlocal character of the electron–photon interaction, which guarantees compliance with the selection rules.
The modeled system is schematically shown Figure 1. We consider a quantum well (QW) between two contacts. The left contact can only inject and collect electrons over an interval of 0.2 eV around the left Fermi level µ_{L}. This value is a bit larger than the broadening of the ground state of the QW, which mimics the IB. Although this is another important issue in IBSC, the optical transition between the valence band and the IB is not treated in this work. In our model we consider this issue solved by assuming the Fermi level µ_{L} located at the maximum of the densityofstates (DOS) of the ground state (middle of the IB). Electrons on this ground state can then interact with photons and reach an excited state. From there, they either relax (and then do not participate in the current) or reach the right contact. This contact, located at an energy E_{c} above µ_{L}, represents the conduction bandedge of the wide bandgap material. By reaching this contact the electrons generate a current that one chooses positive. The right contact can also inject electrons that can reach the QW, relax by emitting a photon and then reach the left contact. This behavior, which corresponds to the relaxation from conduction band to IB, generates a negative current which is all the more important as the right Fermi level µ_{R} is high. In an IBSC the aim is to have a positive current balance (more excitations than relaxations) while having a higher Fermi level in conduction band (µ_{R}) than in IB (µ_{L}). Our system, therefore behaves like an intraband solar cell under bias qV = µ_{R} − µ_{L} and characterized by a current I_{sc} and a voltage V_{oc}. Note finally that, with applied bias, we do not modify the band diagram which is always considered in the flat band approximation.
In the following we compare a boundtobound system in which a tunnel barrier is assumed between the QW and the right contact to a boundtocontinuum system in which we do not assume any barrier. While for an interband transition the definition of the energy gap seems obvious, this is not so trivial for an intrabandone. Instead, we define a threshold energy E_{t} as the resonant energy of the transition between the IB and the conduction band i.e., the energy of the maximum absorption considering a blackbody at 6000 K for the incident photon flux. E_{t} would correspond to the usual energy gap for a system with a steplike absorptivity. For all systems assumed in this work, E_{t} is the same. We chose E_{t} = 1 eV, which is largely compared to what is generally considered in IBSC. This choice is based on a study conducted elsewhere [12] which shows that with a ratchet mechanism [6,13] of 0.7 eV, such a value is optimal in the case where the absorption is rather narrow as expected in intraband system. The other parameter is the effective mass which equals 0.0665 (in free electron mass). Finally we chose to treat a QW since our onedimensional model is well adapted to such a system. However, the physical behaviors, such as confinement and absorption are very close in case of quantum dots. Moreover, if it is straigthforward to add a barrier between a QW and a contact, it is also feasible in case of quantum dots assuming a core–shell architecture [14] or dots embedded in specific material [15]. If in the present study we assume a QW, the conclusions can thus be easily extended to the quantum dots.
Fig. 1 Schematic representation of the modeled system. The fullarrows show the radiative excitation and the collection while the dasharrows represent the injection and the emission. We also show the two Fermi levels µ_{R} and µ_{L}, respectively, corresponding to the IB and the ntype contact. The grey surfaces represent the states. 
3 Results
3.1 Current and voltage with the quantum model
The band diagrams and the localDOS of the two systems are represented in Figure 2. In both the well thickness is 3.2 nm. In one case, the excited state is a localized state separated from the right contact by a 2 nmthick tunnel barrier (Fig. 2a). In this system, called boundtobound (B–B), E_{c} equals 0.88 eV. In the other system the electrons are excited in an energy continuum directly connected to the right contact (Fig. 2b). In the latter case, called boundtocontinuum (B–C), in order to have E_{t} = 1 eV, E_{c} is reduced to 0.855 eV. In Figure 2, the LDOS clearly shows that in B–B the electrons are excited in a localized and narrow quantum state. In B–C, despite the absence of barrier, we do not obtain a true continuum but rather a strongly broadened state. Indeed, even without barrier, the QW involves quantum reflections and then interferences of the electronic wavefunction.
Regarding the results in Figure 2, I_{sc} and V_{oc} are both higher in B–B. In order to understand better the results, Figure 3 shows the electronic current versus the photon energy for the two systems. The absorption spectra corresponds to the positive electronic current while the emission is the negative component. The absorption in B–B is narrower since, as shown in Figure 2, the excited state is thinner. At the same time the current density is much higher than in B–Cʼs counterpart. A higher absorption in B–B structure, as already shown by the intersubband absorption coefficient measured in QWs [8] and theoretically observed in quantum dots [16], is not surprising and is due to a larger wavefunctions overlap. Finally, the higher generated current in B–B is then related to a better tradeoff of the radiative excitation and of the electronic collection. This explains that I_{sc} is larger in B–B despite the tunneling. However, as it will be confirm in the following, a too thick tunnel barrier degrades the current.
From the emission point of view, we obtain lower threshold energy for B–C. As it will be demonstrated in the following, this behavior, which explains the V_{oc} degradation in B–C is related to the broadening of the excited state. This is particularly detrimental when the excited state is a continuum, which is by definition, strongly broadened.
It is possible to improve B–C, for example, by reducing the thickness of the well (2.8 nm). This permits, as shown in Figure 4, to have a quasibound state narrower than the strongly broadened state of the B–C. In this new device, called B–Q, by adjusting E_{c} at 0.88 eV in order to have E_{t} = 1 eV, the current is largely higher than in the original B–C device, while V_{oc} is quite similar. Such a current increase is due to a better excitationcollection tradeoff. However, the current remains lower than in B–B. Moreover, the fact that in B–C and B–Q V_{oc} are close and lower than in B–B, confirms that V_{oc} is not simply controlled by E_{c}. Such results suggest that a narrow excited state is better for V_{oc}. In the following, we propose to use a simpler model in order to verify and explain this counterintuitive feature.
Fig. 2 The banddiagram (white line) and the localDOS of electrons in (a) the boundtobound system and in (b) the boundtocontinuum system. In a corresponding boundtobound IBSC the reduction of voltage due to the presence of the IB should be 1–0.58 = 0.42 V against 1–0.54 = 0.46 V for the boundtocontinuum configuration. 
Fig. 3 Current density versus the photon energy generated in each structure B–B and B–C by (a) photon absorption and (b) photon emission. 
Fig. 4 The banddiagram (white line) and the local DOS of electrons in the boundtoquasibound system. 
3.2 Broadening factor in the detailed balance
We assume a detailed balance model where absorption and emission are calculated assuming a blackbody distribution for the photons and a Lorentzian shape for the electronic DOS. Indeed, if we assume an homogeneous broadening due to contact (or others), the DOS spectral shape of states in the QW is given by a Lorentzian distribution [9]. If the tunneling between the excited state and the contact is low (large lifetime τ) the width Γ of the Lorentzian is low following Γ = ℏ/τ. We then apply this to the DOS of the exited state while, in order to simplify the model, the ground state is assumed as a Dirac function. We finally calculate the current, the emission and the voltage as: (1) (2) (3) with the blackbody distribution (4)and the electronic joined DOS (5)where Γ is the width, E_{t} the energy of the maximum of the Lorentzian, qV = µ_{R} − µ_{L} the bias, k_{B} the Boltzmann constant, and f = C × 6.79 × 10^{−5} with C = 1 the concentration factor. Note that for the integral of A_{b} and E_{m} the minimum of energy is given by E_{c} the bandedge of the right contact. Finally T_{sun} and T_{cell} are respectively the temperature of the sun (6000 K) and of the cell (300 K). In this model the excitationcollection tradeoff is not considered since M^{2}, which represents the optical coupling, is taken as a constant and I_{sc} is directly given by the photon absorption in equation (1). This model is schematically described in Figure 5.
Figure 5 also shows the spectra A_{b} (E) and E_{m} (E) for two values of Γ (5 and 50 meV) with E_{t} = 1 eV and E_{c} = 0.8 eV. As obtained with the NEGF model, and although this detailed balance model does not take into account the excitationcollection tradeoff, we obtain both I_{sc} and V_{oc} larger with a thinner state. As shown in Figure 5, I_{sc} and V_{oc} are even more degraded than the DOS is high in the QW at the bandedge of the contact [L (E_{c}, Γ, E_{t})]. Indeed, a large L (E_{c}, Γ, E_{t}) means that a large proportion of excited electrons cannot be collected since their energy is lower that the bandedge of the contact. This degrades the current. A large L (E_{c}, Γ, E_{t}) also means a large electronic injection from the contact at lowenergy where the emission is very efficient. As already observed in Figure 3, this reduces the energy of the photon emission and then degrades the voltage. Such a behavior, as well as, for example, the reduction of the bandgap by tunneling in ultra thin cells [17], shows that the electronic transport modifies the optical properties of nanoscale devices. Assuming simplified shapes for the functions involved in equations (1) and (2), to analytically solve the corresponding integrals, we obtain this approximate expression for V_{oc}:
With the parameters assumed to calculate the results shown in Figure 5, the equation (7) gives A = 5274 eV^{−1} to be compared to 5800 eV^{−1} for the value found by fitting the numerical data. The two first terms in the expression of V_{oc} are the wellknown Carnot and Boltzmann factors [18,19] while the third one is relative to an original broadening behavior that we call the broadening factor. The origin of this degradation, as already observed in bulk materials [20,21], is the mismatch between the absorption and the emission energies. This factor is generally not considered in detailed balanced [18] since the absorption is assumed sharp at the bandgap. In intraband system this broadening behavior degrades both I_{sc} and V_{oc} when the excited state is too thick like in the boundtocontinuum configuration.
Phonon emission is expected to favor the bandedge photon emission and then to degrade V_{oc}. With our NEGF model we show that such scattering with polar optical phonon is stronger in the continuum than in the QW (and is expected to be even weaker in quantum dot). The consequence is that scattering degrades V_{oc} in B–C (–90 mV) while this degradation is not significant in B–B. This result suggests that scattering with phonon increases the broadening factor. However, this point deserves further investigations, which cannot be conducted in the present work due to huge numerical burden.
Fig. 5 (a) The schematically described detailed balance model and the corresponding I_{sc} and E_{m} spectra for (b) Γ = 5 meV and for (c) Γ = 50 meV. 
3.5 Optimization of the tunnel barrier
The broadening factor may suggest that in the B–B system better characteristics are expected if we assume a thicktunnel barrier between the QW and the contact. Indeed, due to strong tunnel reflection, lifetime increases and then broadening of the excited state decreases. Figure 6 shows the evolution of both I_{sc} and V_{oc} versus the tunnel barrier thickness t_{B} in the B–B system (remember that in Fig. 2a, t_{B} = 2 nm). For t_{B} lower than 2 nm, the reduction of V_{oc} is due to the broadening factor. At the same time the larger current with the ultrathin barrier suggests another behavior like a reduction of the tunnel reflection improving the excitationcollection tradeoff. This is confirmed for the thick barriers where I_{sc} and then the collection are strongly degraded by such a reflection. With a barrier thicker than 3 nm the excitationcollection tradeoff is strongly degraded. In the same time, V_{oc} no more increases for barrier thicker than 2 nm since the excited state is thin enough (≤5 meV) to cancel the broadening factor. For an optimal tunnel barrier both broadening factor and excitationcollection tradeoff should be considered. With the parameters considered in this work the tradeoff is optimal for a 2 nmthick tunnel barrier. In case of a barrier made of an other material with an effective mass m* (in free electron mass) and a rectangular tunnel barrier offset Δ (in eV), this tunneling coupling and then the corresponding excitationcollection tradeoff should be conserved if the thickness of the barrier (in nm) is given by .
Fig. 6 I_{sc}/max (I_{sc}) and V_{oc}/max (V_{oc}) versus the thickness of the tunnel barrier t_{B}. Assuming a thick barrier excited states are very thin and energy mesh has to be also very thin. From a computational point of view we cannot conduct the calculation for tunnel thicker than 3 nm assuming the transverse dispersion. This calculation has then been conducted only for a transverse wave vector equals to zero. 
4 Conclusion
We have shown that a broadening factor degrades the voltage in intraband system by improving the photon emission. To avoid this degradation a boundtobound system in which the electrons are collected by tunneling is well adapted. Moreover, such a thin tunnel barrier improves the excitationcollection tradeoff due to a higher wavefunction overlap. On the other hand, a too thick tunnel barrier degrades this excitationcollection tradeoff due to strong tunnel reflection. It is then necessary to choose a tunnel barrier thick enough to cancel the broadening factor and to improve the wave function overlap, but thin enough to preserve the excitationcollection tradeoff. We finally propose an equation, which allows calculating the thickness of the optimal barrier versus the effective mass and the tunnel barrier offset.
Acknowledgments
Nicolas Cavassilas and Daniel Suchet thank the Japan Society for the Promotion of Science (JSPS) for financial support.
Author contribution statement
N.C. used the homemade quantum transport model developed jointly by N.C., M.B. and F.B.D.S. with N.C. developed the analytical model for the broadening factor. The idea of this study come from discussions at Tokyo University with A.D., J.F.G., M.S. and Y.O. All authors have given approval to the final version of the manuscript.
References
 A. Luque, A. Mart, C. Stanley, Nat. Photon. 6, 146 (2012) [CrossRef] [Google Scholar]
 A. Luque, A. Mart, Phys. Rev. Lett. 78, 5014 (1997) [Google Scholar]
 W. Shockley, H.J. Queisser, J. Appl. Phys. 32, 510 (1961) [Google Scholar]
 T. Sogabe, Y. Shoji, M. Ohba, K. Yoshida, R. Tamaki, H.F. Hong, C.H. Wu, C.T. Kuo, S. Tomi, Y. Okada, Sci. Rep. 4, srep04792 (2014) [Google Scholar]
 Y. Okada, N.J. EkinsDaukes, T. Kita, R. Tamaki, M. Yoshida, A. Pusch, O. Hess, C.C. Phillips, D.J. Farrell, K. Yoshida, et al., Appl. Phys. Rev. 2, 021302 (2015) [Google Scholar]
 A. Pusch, M. Yoshida, N.P. Hylton, A. Mellor, C.C. Phillips, O. Hess, N.J. EkinsDaukes, Progr. Photovoltaics 24, 656 (2016) [CrossRef] [Google Scholar]
 N. López, K.M. Yu, T. Tanaka, W. Walukiewicz, Adv. Energy Mater. 6, 1501820 (2016) [Google Scholar]
 B.F. Levine, A. Zussman, S.D. Gunapala, M.T. Asom, J.M. Kuo, W.S. Hobson, J. Appl. Phys. 72, 4429 (1992) [Google Scholar]
 G. Bastard, Wave mechanics applied to semiconductor heterostructures, in Monographies de Physique (Les Editions de Physique, 1988) [Google Scholar]
 N. Cavassilas, F. Michelini, M. Bescond, J. Renew. Sustain. Energy 6, 011203 (2013) [CrossRef] [Google Scholar]
 N. Cavassilas, F. Michelini, M. Bescond, J. Comput. Electron. 15, 1233 (2016) [Google Scholar]
 A. Delamarre, D. Suchet, M. Sugiyama, N. Cavassilas, Y. Okada, J.F. Guillemoles, Proc. SPIE 10527, 105270R (2018) [Google Scholar]
 M. Yoshida, N.J. EkinsDaukes, D.J. Farrell, C.C. Phillips, Appl. Phys. Lett. 100, 263902 (2012) [Google Scholar]
 S.W. Kim, J.P. Zimmer, S. Ohnishi, J.B. Tracy, J.V. Frangioni, M.G. Bawendi, J. Am. Chem. Soc. 127, 10526 (2005) [Google Scholar]
 D. Sato, J. Ota, K. Nishikawa, Y. Takeda, N. Miyashita, Y. Okada, J. Appl. Phys. 112, 094305 (2012) [Google Scholar]
 S. Tomi, T. Sogabe, Y. Okada, Progr. Photovoltaics 23, 546 (2015) [CrossRef] [Google Scholar]
 U. Aeberhard, U. Rau, Phys. Rev. Lett. 118, 247702 (2017) [CrossRef] [PubMed] [Google Scholar]
 T. Markvart, Phys. Status Solidi a 205, 2752 (2008) [CrossRef] [Google Scholar]
 L.C. Hirst, N.J. EkinsDaukes, Progr. Photovoltaics 19, 286 (2011) [CrossRef] [Google Scholar]
 J. Yao, T. Kirchartz, M.S. Vezie, M.A. Faist, W. Gong, Z. He, H. Wu, J. Troughton, T. Watson, D. Bryant, et al., Phys. Rev. Appl. 4, 014020 (2015) [Google Scholar]
 U. Rau, B. Blank, T.C. Müller, T. Kirchartz, Phys. Rev. Appl. 7, 044016 (2017) [Google Scholar]
Cite this article as: Nicolas Cavassilas, Daniel Suchet, Amaury Delamarre, Fabienne Michelini, Marc Bescond, Yoshitaka Okada, Masakazu Sugiyama, JeanFrancois Guillemoles, Beneficial impact of a thin tunnel barrier in quantum well intermediateband solar cell, EPJ Photovolt. 9, 11 (2018)
All Figures
Fig. 1 Schematic representation of the modeled system. The fullarrows show the radiative excitation and the collection while the dasharrows represent the injection and the emission. We also show the two Fermi levels µ_{R} and µ_{L}, respectively, corresponding to the IB and the ntype contact. The grey surfaces represent the states. 

In the text 
Fig. 2 The banddiagram (white line) and the localDOS of electrons in (a) the boundtobound system and in (b) the boundtocontinuum system. In a corresponding boundtobound IBSC the reduction of voltage due to the presence of the IB should be 1–0.58 = 0.42 V against 1–0.54 = 0.46 V for the boundtocontinuum configuration. 

In the text 
Fig. 3 Current density versus the photon energy generated in each structure B–B and B–C by (a) photon absorption and (b) photon emission. 

In the text 
Fig. 4 The banddiagram (white line) and the local DOS of electrons in the boundtoquasibound system. 

In the text 
Fig. 5 (a) The schematically described detailed balance model and the corresponding I_{sc} and E_{m} spectra for (b) Γ = 5 meV and for (c) Γ = 50 meV. 

In the text 
Fig. 6 I_{sc}/max (I_{sc}) and V_{oc}/max (V_{oc}) versus the thickness of the tunnel barrier t_{B}. Assuming a thick barrier excited states are very thin and energy mesh has to be also very thin. From a computational point of view we cannot conduct the calculation for tunnel thicker than 3 nm assuming the transverse dispersion. This calculation has then been conducted only for a transverse wave vector equals to zero. 

In the text 
Current usage metrics show cumulative count of Article Views (fulltext article views including HTML views, PDF and ePub downloads, according to the available data) and Abstracts Views on Vision4Press platform.
Data correspond to usage on the plateform after 2015. The current usage metrics is available 4896 hours after online publication and is updated daily on week days.
Initial download of the metrics may take a while.